A Slow Leak Synthetic Route to Organically Templated Gallium Sulfates
Kaufman, Elizabeth A.; Zeller, Matthias; Norquist, Alexander J.; Crystal Growth & Design 10 (2010) 4656–; doi:10.1021/cg1009412

data_4502066
_publ_section_title
;
 A Slow Leak Synthetic Route to Organically Templated Gallium Sulfates
;
_journal_issue                   10
_journal_name_full               'Crystal Growth &amp; Design'
_journal_page_first              4656
_journal_paper_doi               10.1021/cg1009412
_journal_volume                  10
_journal_year                    2010
_chemical_formula_moiety         'C6 H26 Ga2 N2 O20 S4'
_chemical_formula_sum            'C6 H26 Ga2 N2 O20 S4'
_chemical_formula_weight         713.98
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_cell_angle_alpha                87.2207(14)
_cell_angle_beta                 82.1832(13)
_cell_angle_gamma                87.5904(13)
_cell_formula_units_Z            1
_cell_length_a                   5.6262(7)
_cell_length_b                   8.9854(10)
_cell_length_c                   10.3386(12)
_cell_measurement_reflns_used    4606
_cell_measurement_temperature    110
_cell_measurement_theta_max      31.3067
_cell_measurement_theta_min      2.9546
_cell_volume                     516.86(11)
_computing_cell_refinement       APEX2
_computing_data_collection       APEX2
_computing_data_reduction        APEX2
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'SIR92 (Altomare et al., 1993)'
_diffrn_ambient_temperature      100
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.902
_diffrn_measurement_device       'Bruker AXS Smart Apex CCD'
_diffrn_measurement_device_type  Area
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.015
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -7
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            8807
_diffrn_reflns_theta_full        25.703
_diffrn_reflns_theta_max         31.345
_diffrn_reflns_theta_min         2.271
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    3.115
_exptl_absorpt_correction_T_max  0.73
_exptl_absorpt_correction_T_min  0.73
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'DENZO/SCALEPACK (Otwinowski & Minor, 1997)'
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    2.294
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             362
_exptl_crystal_size_max          0.400
_exptl_crystal_size_mid          0.250
_exptl_crystal_size_min          0.15
_refine_diff_density_max         0.55
_refine_diff_density_min         -0.44
_refine_ls_extinction_coef       10.7(15)
_refine_ls_extinction_method     'Larson (1970), Equation 22'
_refine_ls_goodness_of_fit_ref   1.0171
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     155
_refine_ls_number_reflns         2964
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0182
_refine_ls_R_factor_gt           0.0177
_refine_ls_shift/su_max          0.0019565
_refine_ls_shift/su_mean         0.0003548
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 Method= Modified Sheldrick 
 w=1/[\s^2^(F^2^) + ( 0.03P)^2^ + 0.46P] 
 ,where P=(max(Fo^2^,0) + 2Fc^2^)/3 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.0508
_refine_ls_wR_factor_gt          0.0484
_refine_ls_wR_factor_ref         0.0481
_reflns_limit_h_max              7
_reflns_limit_h_min              -7
_reflns_limit_k_max              13
_reflns_limit_k_min              -12
_reflns_limit_l_max              15
_reflns_limit_l_min              0
_reflns_number_gt                3008
_reflns_number_total             3072
_reflns_threshold_expression     I>2.0\s(I)
_oxford_diffrn_Wilson_B_factor   0.44
_oxford_diffrn_Wilson_scale      1.76
_oxford_refine_ls_r_factor_ref   0.0175
_oxford_refine_ls_scale          0.7663(14)
_oxford_reflns_number_all        3066
_oxford_reflns_threshold_expression_ref I>3.0\s(I)
_cod_data_source_file            cg1009412_si_001.cif
_cod_data_source_block
'[C~6~H~18~N~2~][Ga(H~2~O)~2~(SO~4~)~2~]~2~_Cmp-4'
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Triclinic' changed to 'triclinic'
according to /home/saulius/struct/CIF-dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 1715 2011-07-08 13:25:40Z adriana 
;
_cod_original_sg_symbol_H-M      'P -1 '
_cod_database_code               4502066